Bio-inspired strategies for designing antifouling biomaterials
© The Author(s). 2016
Received: 18 March 2016
Accepted: 2 June 2016
Published: 20 June 2016
Contamination of biomedical devices in a biological medium, biofouling, is a major cause of infection and is entirely avoidable. This mini-review will coherently present the broad range of antifouling strategies, germicidal, preventive and cleaning using one or more of biological, chemical and physical techniques. These techniques will be discussed from the point of view of their ability to inhibit protein adsorption, usually the first step that eventually leads to fouling. Many of these approaches draw their inspiration from nature, such as emulating the nitric oxide production in endothelium, use of peptoids that mimic protein repellant peptides, zwitterionic functionalities found in membrane structures, and catechol functionalities used by mussel to immobilize poly(ethylene glycol) (PEG). More intriguing are the physical modifications, creation of micropatterns on the surface to control the hydration layer, making them either superhydrophobic or superhydrophilic. This has led to technologies that emulate the texture of shark skin, and the superhyprophobicity of self-cleaning textures found in lotus leaves. The mechanism of antifouling in each of these methods is described, and implementation of these ideas is illustrated with examples in a way that could be adapted to prevent infection in medical devices.
KeywordsAntifouling Bio-inspired Biomaterials Nitric oxide Hydration Peptoids PEG DOPA Zwitterions Micropatterning
Biofouling is the contamination of surfaces by microbes that include bacteria (prokaryotes), fungi and viruses. In medical applications, biofouling occurs on surgical equipment, protective apparel, packaging, guide wires, sensors, prosthetic devices, and medical implants, and most familiarly on catheters, drug delivery devices and contact lenses. Microbial contamination, and the subsequent risk of infection, biosensor failure and implant rejection, is a major driver in developing efficient antifouling strategies . According to a recent study initiated by the Centers for Disease Control and Prevention, about 26 % of the health-care related infections are caused by these device-associated infections in U.S. acute care hospitals alone in 2011 . Prevention of morbidity and mortality associated with biofilm-mediated infections calls for the replacement of contaminated devices, as well as treatment with antibiotics, which sometimes may be ineffective .
Since biofouling is mediated by proteins, inhibition of protein adsorption prevents the cause of infection at the source. The layer of adsorbed protein on surfaces serves as a platform for cell attachment, and subsequent bacterial colonization that leads to the formation of bacterial films . Protein fouling is a major challenge in the development of numerous blood-contacting biomedical devices caused by the nonspecific adhesion of biological components including proteins to the device surface. These pro-inflammatory processes result in thrombus formation, which leads to platelet formation, and ultimately to device failures and fatal complications. There are many excellent reviews [5–7] on antifouling strategies for a wide variety of applications, marine, industrial (e.g., reverse osmosis membranes), and biomedical applications [8–12]. We distinguish our review from these by focusing on biomedical devices and discuss a broad range of possible methods, biological, chemical and physical, in sufficient detail.
Strategies for making antifouling biomedical surfaces
There are three strategies: First is the use of biocides, antibacterials that kill bacteria or antimicrobial that kill bacteria and other microorganisms. Second is to repel the proteins, and subsequently cells, and thus prevent biofouling. Third is to create surfaces that self-clean so that the organisms do not remain attached. Nature appears to have developed a combination of these approaches.
Comparison of various antifouling strategies presented in this paper
1. Biological molecules
1.1 Nitric oxide-releasing materials
Oxidative or nitrosative stress-inducing moieties are produced within the biofilm structure to cause bacteriophage induction, and cell lysis.
Synthetic NO donor supplements the natural sources
Because of high reactivity (instability), storage and delivery requires special attention.
Selective to only certain bacterial types.
1.2 Peptide and peptoid modified surfaces
Through structural reformations that inhibit cell adhesion.
Exceptional resistance to a wide variety of proteins.
High cost of peptide/peptoid modification of surfaces
Tailorable surface structure for optimum performance.
2. Chemical modification
2.1 Hydrophilic polymers
A layer of strongly bound water that cannot be displaced by a protein and thus inhibiting protein adsorption.
Uses poly(ethylene glycol) (PEG), an U.S. federal drug administration (FDA) approved GRAS (generally recognized as safe) substance
Oxidative damages and low surface densities limit long-term application.
2.2 Immobilization of PEG
Anchoring of PEG using a mussel-mimicking linker.
Less susceptible to hydrolytic degradation than free PEG
Limited by the availability of suitable surface functionalities for anchoring PEG
2.3 Zwitterionic polymers
High protein resistance through the formation of “super-hydrophilicity”.
Long-term antifouling characteristics.
Limited commercial availability of zwitterionic polymers
Unique capability for ligand immobilization.
2.4 Hydrophobic polymers
Inhibits the adsorption of proteins that require polar surfaces.
Many hydrophobic polymers are commercially available.
Toxicity concerns with many hydrophobic polymers.
3. Micropatterning of surfaces
Self-cleaning ability of the superhydrophobic surface prevents adhesion
A physical texture enhances the role of the simple waxy surface
Limited by fabrication techniques and general applicability
3.2 Shark-skin patterns
Surface patterns along with an antifouling chemical agent sloughs of attached cells
A physical modification of the surface to enhance the effect of chemical agent
Limited by wide applicability. Applicable to moving surfaces.
Use of biological molecules
Use of biological molecules for antifouling applications are attractive as these are naturally occurring biomolecules or entities that are inherently less toxic, more efficient, and have greater specificity than many synthetic compounds . Three of the most promising molecules are nitric-oxide releasing materials, peptides and peptoids.
Nitric oxide-releasing materials
Initial studies using the NO-donor sodium nitroprusside (SNP) have shown that use of sub lethal concentrations (25 to 500 nM) of the NO-donor resulted in a significant dispersal of bacterial biofilms (Pseudomonas aeruginosa) . In another study, researchers demonstrated that NO released from the donor PROLI/NO (1-[2-(carboxylato)-pyrrolidin-1-yl]diazen-1-ium-1,2-diolate) resulted in nearly 66 % reduction in proteins and nearly 50 % reduction in the biofilm surface coverage compared to the untreated control . Similarly, using another NO-donor, S-nitroso-N-acetylpenicilamine (SNAP), Brisbois et al. successfully demonstrated a 90 % reduction in bacterial adhesion and infection by NO-releasing materials in a 7 days animal model .
Although NO can be an effective molecule for the prevention of biofilm formation and biofilm-related infections, its use in many biomedical applications remains a challenge because of high reactivity and short half-life, its requirement for proper storage and delivery. Covalent incorporation of a suitable NO-donor during the synthesis or impregnating it into a suitable matrix during the processing are some of the approaches reported to date for modulating the NO-release towards biomedical applications [22–25]. One other limitation with the NO approach is that in certain instances NO was found to have no influence, and even stimulate biofilm formation in certain types of bacterial colonies [26–28]. Consequently, NO may be used selectively for controlling the biofilm formation in certain types of bacteria. Since there is a large range of biofilm responses, detailed research is required to establish the generalized use of NO over a variety of non-fouling applications.
Peptide and peptoid modified surfaces
Many peptide-based materials are used as antifouling agents because of their exceptional resistance to proteins including bovine serum albumin, fibrinogen, fibronectin, lysozyme, and streptavidin [29, 30]. Naturally occurring biomolecule such as amino acids, peptides, and polysaccharides are also commonly used in the development of innovative antifouling materials. Many of these biomolecules are believed to undergo structural reformations under physiological conditions to prevent biofouling . Peptoids are non-natural biomimetic polymers. Unlike poly(ethylene glycol) (PEG) and zwitterions that will be discussed shortly, the surface structure and antifouling ability of the peptide- and peptoid-based materials can be tuned [31, 32]. Many known antifouling functionalities can be incorporated using a single backbone chemistry, and done so at precisely known locations, because of the sequence specificity of polypeptoids. A library of such sequence-specific materials can be designed for optimum performance.
In one example, a biomimetic antifouling material was prepared by Perrino et al.  by grafting dextran side chain to a poly(L-lysine) (PLL) backbone. The PLL-graft-dextran copolymer was found to have excellent antifouling properties to prevent nonspecific adsorption of proteins in a variety of architectures similar to a PEG-grafted analog. A similar biomolecule-based approach is to incorporate proteases onto the material surfaces. In one such attempt, Kim et al.  prepared protein resistant films by immobilizing hydrolytic enzymes pronase and α-chymotrypsin by sol–gel entrapment followed by covalent attachment to a polydimethylsiloxane (PDMS) matrix.
Chemical modification of surfaces
Unlike the approaches discussed in a previous section, need exists for non-specific protein repulsion. This can be achieved by incorporating hydrophilic polymers such as PEG, amphiphilic fluoropolymers, zwitterionic polymers . Chen et al. have summarized these polymers under two major classes, polyhydrophilic and poly zwitterionic . While hydrophilic polymers resist protein adsorption by forming a hydration layer, hydrophobic surfaces prevent fouling by being able to readily release the adsorbed proteins and cells. All these polymers can be applied onto a variety of surfaces by one of many physical techniques such as spin-coating and dip-coating, or chemical methods such as covalent grafting. We will discuss the application of some of these polymers to biomedical devices.
Surface modification with PEG is widely used in preventing biofouling on medical devices . Each ethylene glycol repeating unit in the PEG backbone can strongly bind to one water molecule, bridging the ether oxygen along the 72 helical PEG chain [40–42]. This unique interaction between the water and the PEG chain results in the formation of a highly hydrated layer and ultimately leads to a steric hindrance to the approaching protein molecules . When a protein molecule approaches a hydration layer barrier, the resulting compression of the layer can decrease the conformational entropy of the polymer chains that ultimately lead to the repulsion of the approaching proteins. Such a hydration layer does not occur in polyoxymethylene even with its higher O/C ratio. High mobility and large exclusion volume of the PEG chains also contribute towards the overall antifouling characteristics of the polymer.
Despite the attractiveness of PEG as an antifouling agent, low surface densities [43, 44] and susceptibility to oxidative damages  limit their antifouling capabilities overlong-term applications. Additionally, it has been shown that reactive oxygen species, produced by PEG might modulate the cell response . For these reasons, alternate hydrophilic polymers such as polyglycerols , polyoxazolines , polyamides , and naturally occurring polysaccharides  have been evaluated for antifouling applications.
Immobilization of PEG
A surface can be functionalized with PEG by using either adsorption of presynthesized PEG onto the surface (graft-to strategy), or by growing the polymer in-situ via surface adsorbed initiation group (graft-from strategy) . Both of these techniques immobilize PEG on surfaces to confer them with protein and cell resistance. However, anchoring PEG by using functional groups on the surface requires extensive chemical modification of the surface, especially to make them less susceptible to thermal and hydrolytic degradation, and is therefore limited by the surface chemistry.
Following nature’s cues, PEG can be robustly anchored onto a variety of surfaces using a mussel-mimicking linker, adhesive L-3,4-dihydroxyphenylalanine (DOPA), a catechol functionality . DOPA, DOPA peptides, or a catechol-mimic molecule can be covalently attached to the PEG terminal hydroxyl groups or to side chains. Alternatively, DOPA or a catechol-based monomer can be directly incorporated into the polymer backbone during polymerization. The catechol segment imparts the cohesive and adhesive characteristics, while PEG contributes to the antifouling characteristics .
Zwitterionic materials are amphoteric materials with both positive and negative charges. Because of the strong dipoles of the zwitterions and electrostatic itneractions, they have a stongly bound hydration layer that leads to “superhydrophilicity” and high protein resistivity . Consequently, the extent of nonfouling characteristics exhibited by this group of materials is greater than that observed with hydrophilic/hydrophobic materials. Zwitterionic phospholipids such as phosphorylcholine constitute the outer surface of the nonthrombogenic erythrocyte cell membranes [56, 57]. Inspired by the antifouling properties of these naturally occurring membrane molecules, researchers have explored the potential utility of zwitterionic polymeric materials such as polybetaines or its structural analogs in a variety of biomedical applications, including nonthrombogenic surfaces .
An early example of bio-membrane mimicry is the preparation of phosphobetaine (PB)-based antifouling surfaces by incorporating the structural analogs of the naturally occurring lipid dipalmitoyl phosphatidylcholine (DPPC), such as diacetylenic phosphatidylcholine (DAPC) and methacryloyloxyalkyl phosphorylcholines (MAPC) [59–62]. Because of the characteristic ability of the phosphobetaines to retain a large amount of water with the zwitterionic head groups while retaining protein repulsion, PB-modified hydrogels are finding their importance in contact lens applications for improving the wettability and surface properties .
Other polybetaines, such as carboxybetaines (CB) and sulfobetaines (SB) are also been extensively evaluated for various nonfouling biomedical applications. Among these, CB is attractive because of its unique capability for immobilizing ligands such as proteins and antibodies, onto the carboxyl groups [64, 65]. Cheng et al. used a cationic precursor of poly(carboxybetaine methacrylate) (polyCBMA) to produce a switchable polymer surface coating with self-sterilizing and nonfouling capabilities [66, 67]. The cationic precursor of polyCBMA killed more than 99.9 % of Escherichia coli K 12 in 1 h and upon hydrolysis switched to a zwitterionic nonfouling surface with the release of more than 98 % of the dead bacterial cells and prevented any further protein attachment and biofilm formation.
Like many carboxybetaines, densely packed poly(sulfobetaine methacrylate) (polySBMA)-grafted surfaces have also been found to be completely resistant to the adsorption of a number of plasma proteins including human serum albumin, gamma globulin, fibrinogen, and lysozyme, even at low ionic concentrations [68–70]. PolyCBMA is also an interesting polymer for making blood-compatible surfaces, because of its structural comparability with the naturally occurring glycine betaine. Furthermore, the surface carboxyl groups polyCBMA provide a suitable platform for covalent immobilization of bioactive species such as monoclonal mouse antibody (mAb, anti-hCG) for specifically binding to human chorionic gonadotropin (hCG) while retaining the nonspecific protein repellency . This dual functional behavior of polyCBMA makes it useful for the design of antifouling surfaces for biosensors and diagnostic applications.
Hydrophobic coatings have been developed in textile industry to prevent staining . These coating are effective as fouling release agents. In one study, Privett et al. reported the development of a superhydrophobic xerogel coating synthesized from a mixture of nanostructured fluorinated silica colloids, fluoroalkoxysilane, and a backbone silane . The researchers showed a significant reduction in the adhesion of Staphylococcus aureus and Pseudomonas aeruginosa (P. aeruginosa.) on this fluorinated surface compared to their control samples. In another example, Li et al.  used a hydrophobic liquid-infused porous poly(butyl methacrylate-co-ethylene dimethacrylate) surface (slippery BMA-EDMA) for reducing the adhesion of P. aeruginosa. Only ~1.8 % of the slippery surface was covered by the environmental P. aeruginosa PA49 strain whereas the uncoated glass controls exhibited coverage of ~55 % under the same conditions. However, mainly due to the toxicity concerns, the hydrophobic polymers are not studied as extensively as their hydrophilic analogs.
Recently, Xue et al. reported the development of superhydrophobic antifouling poly(ethylene terephthalate) (PET) fabrics by chemical etching followed by grafting of fluorinated methacrylate polymers via surface-initiated atom radical polymerization (SI-ATRP) . The hydrophobicity of the surfaces were controlled by tuning the polymerization time and a contact angle of nearly 160 ° was reported by the researchers after 8 h with excellent antifouling properties. Since PET is extensively used in a variety of biomedical applications, this innovative approach can be adapted to improve the antifouling properties of many currently available biomedical devices.
Micropatterning of surfaces
Influence of surface texture
It has been known for more than 100 years that cell response is influenced by surface topology . Investigations over the past 50 years have demonstrated that surface topography in the μm length scale affects the cell adhesion [76–81]. Many of these investigations were carried out in the context to cell survival and promotion of cell growth. Recent work has shown that such surface topography can be used reduce biofilm formation . The discovery that such topography is in fact used by marine species to prevent biofouling has inspired the development of strategies for developing similar surfaces on biomedical devices [10, 83]. Topographical features suitable for controlling cell adhesion are traditionally produced by photolithography . Alternative approaches include demixing [84–86], dewetting , solvent evaporation , and laser ablation . These and other techniques can produce micro-topographies found on leaves on many plants, most well known being lotus, and dermal denticles on skins of marine organisms such as shark, whales, bottlenose dolphin mussels, snail shells, and edible crab.
The mechanisms by which the naturally occurring micro-topographic features prevent biofilm formation are still not clear. There are at least four mechanisms that contribute to the antifouling properties of the surface. In one mechanism, the lotus effect, superhydrophobity of the surface causes water to bead up on the surface, and pick up the contaminants as it rolls off the surface, and thus prevent attachment of any cells onto the surface [11, 89]. In the second mechanism, the topography is such that it prevents cellular attachment [90, 91]. In the third, the drag and the efficient flow of water, sloughs off the organism of the surface . According to the fourth mechanism, marine animals secrete substances contribute to the antifouling properties of these surfaces [83, 92]. Irrespective of the mechanisms, these bioinspired structures, since they do not alter the chemical composition or add extraneous chemical into the mix, have found potential use in applications such as catheters . We will discuss two bioinspired micropatterns that highlight this class of structures.
Superhydrophobic self-cleaning surfaces
It should be noted, that the 2nd level of wax-like hairy is important for the superhydrophobicity of the surface. There are cone-like structures that lack the hair features present on the cones of lotus leaf. As a consequence, a droplet of water spreads on these leaves. Such structures are present on the leaves of plants such as Calathea Zebra . The structure shown in Fig. 5b mimics these hair-less cones, and was obtained laser ablation of a polyester film . These structures are formed by self-assembly, and can thus be formed on any complex surface found on medical devices.
Topography driven antifouling
Although Micropatterned surfaces by themselves have been shown to reduce the transfer of bacterial contamination , there are other reports that suggest additional chemical modification may be necessary to achieve the desired level of antifouling . For instance, mucous found on the shark skin also provides lubricating and antifouling benefits . In another study, decoupling the surface chemistry from the topography lead to fouling of such surface during 3 to 6 weeks of immersion . Such studies show that topographical features and surface properties can play a major role in designing antifouling surfaces for innovative biomedical surfaces .
The surface patterning involves surface modification via nanoparticles, photolithography, mesoporous polymers, or surface etching, sometimes in conjunction with additional chemical modifications to reduce surface energy. These often require harsh synthetic conditions complex fabrication techniques [89, 102, 103] thus limiting the substrate type and geometry that may be coated.
Antifouling can be achieved by mimicking the strategies developed by nature instead of using synthetic antimicrobials and antibiotics. We have presented several strategies that can be adopted on biomedical devices and a comparative summary of various methods is presented in Table 1. Nitric oxide (NO) releasing agents are based on processed used by endothelium. Peptides and peptoids use specific protein repulsion approaches. There are widely successful approaches based on hydration layer that uses hydrophilic polymers such PEG and zwitterions. Several micropatterning approaches that mimic the surfaces of plant leaves and skins of marine animals are also discussed. These methods suggest the many ways in which the formation of biofilms on the material surface can be prevented in various biomedical devices particularly for blood-contacting biomedical applications.
BMA-EDMA, poly(butyl methacrylate-co-ethylene dimethacrylate); CB, carboxybetaine; c-di-GMP, cyclic diguanylate; DAPC, diacetylenic phosphatidylcholine; DOPA, 3,4-dihydroxyphenylalanine; DPPC, dipalmitoyl phosphatidylcholine; hCG, human chorionic gonadotropin; mAb, monoclonal antibody; MAPC, methacryloyloxyalkyl phosphorylcholine; NO, Nitric oxide; P. aeruginosa, Pseudomonas aeruginosa; PB, phosphobetaine; PDMS, polydimethylsiloxane; PDN-PEG, poly[(N,N-dimethylacrylamide)15-co-(N-3,4-dihydroxyphenethyl acrylamide)2]-b-poly(ethylene glycol)45; PEG, poly(ethylene glycol); PET, poly(ethylene terephthalate); PLL, poly(L-lysine); PMP1, a peptidomimetic peptide-peptoid based material; polyCBMA, poly(carboxybetaine methacrylate); polySBMA, poly(sulfobetaine methacrylate); PROLI/NO, 1-[2-(carboxylato)-pyrrolidin-1-yl]diazen-1-ium-1,2-diolate; S. woodyi, Shewanella woodyi; SB, sulfobetaine; SI-ATRP, surface-initiated atom radical polymerization; SNAP, S-nitroso-N-acetylpenicilamine; SNP, sodium nitroprusside; SwDGC, diguanylate cyclase gene of S. woodyi; SwH-NOX, S. woodyi with heme-nitric oxide/oxygen binding
Availability of data and materials
No original data are reported in this article.
VBD researched and wrote the chemical-modification sections. NSM chose the topics, researched and wrote the physical-modification sections, and revised the final manuscript. Both authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Ethics approval and consent to participate
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Chan J, Wong S. Biofouling: Types, Impact, and Anti-fouling. New York: Nova Science Publishers; 2010.Google Scholar
- Magill SS et al. Multistate point-prevalence survey of health care–associated infections. N Engl J Med. 2014;370(13):1198–208.View ArticleGoogle Scholar
- Lehman SM, Donlan RM. Bacteriophage-mediated control of a two-species biofilm formed by microorganisms causing catheter-associated urinary tract infections in an in vitro urinary catheter model. Antimicrob Agents Chemother. 2015;59(2):1127–37.View ArticleGoogle Scholar
- Costerton JW, Montanaro L, Arciola CR. Biofilm in implant infections: Its production and regulation. Int J Artif Organs. 2005;28(11):1062.Google Scholar
- Banerjee I, Pangule RC, Kane RS. Antifouling coatings: recent developments in the design of surfaces that prevent fouling by proteins, bacteria, and marine organisms. Adv Mater. 2011;23(6):690–718.View ArticleGoogle Scholar
- Krishnan S, Weinman CJ, Ober CK. Advances in polymers for anti-biofouling surfaces. J Mater Chem. 2008;18(29):3405–13.View ArticleGoogle Scholar
- Zhou F. Antifouling Surfaces and Materials. Berlin: Springer; 2014.Google Scholar
- Xiong Y, Liu Y. Biological control of microbial attachment: a promising alternative for mitigating membrane biofouling. Appl Microbiol Biotechnol. 2010;86(3):825–37.View ArticleGoogle Scholar
- Malaeb L, et al. Do biological-based strategies hold promise to biofouling control in MBRs? Water Res. 2013;47(15):5447–63.View ArticleGoogle Scholar
- Salta M, et al. Designing biomimetic antifouling surfaces. Philos T Roy Soc A. 2010;368(1929):4729–54.View ArticleGoogle Scholar
- Bixler GD, Bhushan B. Biofouling: lessons from nature. Philos T Roy Soc A. 2012;370(1967):2381–417.View ArticleGoogle Scholar
- Bixler GD, et al. Anti-fouling properties of microstructured surfaces bio-inspired by rice leaves and butterfly wings. J Colloid Interface Sci. 2014;419:114–33.View ArticleGoogle Scholar
- Ignarro LJ, et al. Endothelium-derived relaxing factor produced and released from artery and vein is nitric oxide. Proc Natl Acad Sci. 1987;84(24):9265–9.View ArticleGoogle Scholar
- Barraud N, et al. Involvement of nitric oxide in biofilm dispersal of pseudomonas aeruginosa. J Bacteriol. 2006;188(21):7344–53.View ArticleGoogle Scholar
- Damodaran VB, et al. S-Nitrosated biodegradable polymers for biomedical applications: synthesis, characterization and impact of thiol structure on the physicochemical properties. J Mater Chem. 2012;22(13):5990–6001.View ArticleGoogle Scholar
- Damodaran VB, Reynolds MM. Nitric oxide-releasing biomedical materials. In: Mishra MK, editor. Encyclopedia of biomedical polymers and polymeric biomaterials. NY: Taylor & Francis; 2015. doi:10.1081/E-EBPP-120049951.Google Scholar
- Damodaran VB, et al. Antithrombogenic properties of a nitric oxide-releasing dextran derivative: evaluation of platelet activation and whole blood clotting kinetics. RSC Advances. 2013;3(46):24406–14.View ArticleGoogle Scholar
- Liu N, et al. Nitric oxide regulation of cyclic di-GMP synthesis and hydrolysis in Shewanella woodyi. Biochemistry. 2012;51(10):2087–99.View ArticleGoogle Scholar
- Barnes RJ, et al. Nitric oxide treatment for the control of reverse osmosis membrane biofouling. Appl Environ Microbiol. 2015;81(7):2515–24.View ArticleGoogle Scholar
- Brisbois EJ, et al. Reduction in thrombosis and bacterial adhesion with 7 day implantation of S-nitroso-N-acetylpenicillamine (SNAP)-doped Elast-eon E2As catheters in sheep. J Mater Chem B. 2015;3(8):1639–45.View ArticleGoogle Scholar
- Barraud N, et al. Cephalosporin-3′-diazeniumdiolates: targeted NO-donor prodrugs for dispersing bacterial biofilms. Angewandte Chemie. 2012;124(36):9191–4.View ArticleGoogle Scholar
- Damodaran VB, et al. Enzymatically degradable nitric oxide releasing S-nitrosated dextran thiomers for biomedical applications. J Mater Chem. 2012;22(43):23038–48.View ArticleGoogle Scholar
- Koh A, et al. Nitric oxide-releasing silica nanoparticle-doped polyurethane electrospun fibers. ACS Appl Mater Interfaces. 2013;5(16):7956–64.View ArticleGoogle Scholar
- Colletta A, et al. S-Nitroso-N-acetylpenicillamine (SNAP) impregnated silicone foley catheters: a potential biomaterial/device to prevent catheter-associated urinary tract infections. ACS Biomaterials Science & Engineering. 2015;1(6):416–24.View ArticleGoogle Scholar
- Joslin JM, Damodaran VB, Reynolds MM. Selective nitrosation of modified dextran polymers. RSC Advances. 2013;3(35):15035–43.View ArticleGoogle Scholar
- Zaitseva J, et al. Effect of nitrofurans and NO generators on biofilm formation by Pseudomonas aeruginosa PAO1 and Burkholderia cenocepacia 370. Res Microbiol. 2009;160(5):353–7.View ArticleGoogle Scholar
- Schmidt I, et al. Physiologic and proteomic evidence for a role of nitric oxide in biofilm formation by nitrosomonas europaea and other ammonia oxidizers. J Bacteriol. 2004;186(9):2781–8.View ArticleGoogle Scholar
- Arruebarrena Di Palma A, et al. Denitrification-derived nitric oxide modulates biofilm formation in Azospirillum brasilense. FEMS Microbiol Lett. 2013;338(1):77–85.View ArticleGoogle Scholar
- Chelmowski R, et al. Peptide-based SAMs that resist the adsorption of proteins. J Am Chem Soc. 2008;130(45):14952–3.View ArticleGoogle Scholar
- Chen S, Cao Z, Jiang S. Ultra-low fouling peptide surfaces derived from natural amino acids. Biomaterials. 2009;30(29):5892–6.View ArticleGoogle Scholar
- Leng C, et al. Surface structure and hydration of sequence-specific amphiphilic polypeptoids for antifouling/fouling release applications. Langmuir. 2015;31(34):9306–11.View ArticleGoogle Scholar
- van Zoelen W, et al. Sequence of hydrophobic and hydrophilic residues in amphiphilic polymer coatings affects surface structure and marine antifouling/fouling release properties. ACS Macro Letters. 2014;3(4):364–8.View ArticleGoogle Scholar
- Perrino C, et al. A biomimetic alternative to poly(ethylene glycol) as an antifouling coating: resistance to nonspecific protein adsorption of poly(l-lysine)-graft-dextran. Langmuir. 2008;24(16):8850–6.View ArticleGoogle Scholar
- Kim YD, Dordick JS, Clark DS. Siloxane-based biocatalytic films and paints for use as reactive coatings. Biotechnol Bioeng. 2001;72(4):475–82.View ArticleGoogle Scholar
- Mason JM. Design and development of peptides and peptide mimetics as antagonists for therapeutic intervention. Future Med Chem. 2010;2(12):1813–22.View ArticleGoogle Scholar
- Statz AR, et al. New peptidomimetic polymers for antifouling surfaces. J Am Chem Soc. 2005;127(22):7972–3.View ArticleGoogle Scholar
- Lin S, et al. Antifouling poly(β-peptoid)s. Biomacromolecules. 2011;12(7):2573–82.View ArticleGoogle Scholar
- Chen S, et al. Surface hydration: principles and applications toward low-fouling/nonfouling biomaterials. Polymer. 2010;51(23):5283–93.View ArticleGoogle Scholar
- Harris JM. Poly (ethylene glycol) chemistry: biotechnical and biomedical applications. Berlin: Springer Science & Business Media; 1992.Google Scholar
- Lüsse S, Arnold K. The interaction of poly(ethylene glycol) with water studied by 1H and 2H NMR relaxation time measurements. Macromolecules. 1996;29(12):4251–7.View ArticleGoogle Scholar
- Oesterhelt F, Rief M, Gaub H. Single molecule force spectroscopy by AFM indicates helical structure of poly (ethylene-glycol) in water. New J Phys. 1999;1(1):6.View ArticleGoogle Scholar
- Aray Y, et al. Electrostatics for exploring the nature of the hydrogen bonding in polyethylene oxide hydration. J Phys Chem B. 2004;108(7):2418–24.View ArticleGoogle Scholar
- Kingshott P, et al. Covalent attachment of poly(ethylene glycol) to surfaces, critical for reducing bacterial adhesion. Langmuir. 2003;19(17):6912–21.View ArticleGoogle Scholar
- Damodaran VB, Fee CJ, Popat KC. Prediction of protein interaction behaviour with PEG-grafted matrices using X-ray photoelectron spectroscopy. Appl Surf Sci. 2010;256(16):4894–901.View ArticleGoogle Scholar
- Ostuni E, et al. A survey of structure–property relationships of surfaces that resist the adsorption of protein. Langmuir. 2001;17(18):5605–20.View ArticleGoogle Scholar
- Sung H-J, et al. Poly (ethylene glycol) as a sensitive regulator of cell survival fate on polymeric biomaterials: the interplay of cell adhesion and pro-oxidant signaling mechanisms. Soft Matter. 2010;6(20):5196–205.View ArticleGoogle Scholar
- Weber T, et al. Direct grafting of anti-fouling polyglycerol layers to steel and other technically relevant materials. Colloids Surf B Biointerfaces. 2013;111:360–6.View ArticleGoogle Scholar
- Konradi R, Acikgoz C, Textor M. Polyoxazolines for nonfouling surface coatings — a direct comparison to the gold standard PEG. Macromol Rapid Commun. 2012;33(19):1663–76.View ArticleGoogle Scholar
- Lopez AI, et al. Biofunctionalization of silicone polymers using poly(amidoamine) dendrimers and a mannose derivative for prolonged interference against pathogen colonization. Biomaterials. 2011;32(19):4336–46.View ArticleGoogle Scholar
- Gölander C-G, et al. Properties of immobilized PEG films and the interaction with proteins, in Poly (ethylene glycol) Chemistry. Berlin: Springer; 1992. p. 221–45.Google Scholar
- Dalsin JL, et al. Mussel adhesive protein mimetic polymers for the preparation of nonfouling surfaces. J Am Chem Soc. 2003;125(14):4253–8.View ArticleGoogle Scholar
- Lee BP, et al. Mussel-inspired adhesives and coatings. Annu Rev Mater Res. 2011;41(1):99–132.View ArticleGoogle Scholar
- Li L, et al. Mussel-inspired antifouling coatings bearing polymer loops. Chem Commun. 2015;51(87):15780–3.View ArticleGoogle Scholar
- Kang T, et al. Mussel-inspired anchoring of polymer loops that provide superior surface lubrication and antifouling properties. ACS Nano. 2016;10(1):930–7.View ArticleGoogle Scholar
- Damodaran VB, et al. Zwitterionic polymeric materials. In: Mishra MK, editor. Encyclopedia of biomedical polymers and polymeric biomaterials. NY: Taylor & Francis; 2015. doi:10.1081/E-EBPP-120050037.Google Scholar
- Zwaal RFA, Schroit AJ. Pathophysiologic implications of membrane phospholipid asymmetry in blood cells. Blood. 1997;89(4):1121–32.Google Scholar
- Zwaal RFA, Comfurius P, Van Deenen LLM. Membrane asymmetry and blood coagulation. Nature. 1977;268(5618):358–60.View ArticleGoogle Scholar
- Lewis AL. Phosphorylcholine-based polymers and their use in the prevention of biofouling. Colloids Surf B Biointerfaces. 2000;18(3–4):261–75.View ArticleGoogle Scholar
- Hall B, et al. Biomembranes as models for polymer surfaces: V. Thrombelastographic studies of polymeric lipids and polyesters. Biomaterials. 1989;10(4):219–24.View ArticleGoogle Scholar
- Hayward JA, et al. Biomembpanes as models for polymer surfaces. Biomaterials. 1986;7(2):126–31.View ArticleGoogle Scholar
- Ishihara K, et al. Modification of polysulfone with phospholipid polymer for improvement of the blood compatibility. Part 1. Surface characterization. Biomaterials. 1999;20(17):1545–51.View ArticleGoogle Scholar
- Kojima M, et al. Interaction between phospholipids and biocompatible polymers containing a phosphorylcholine moiety. Biomaterials. 1991;12(2):121–4.View ArticleGoogle Scholar
- Willis SL, et al. A novel phosphorylcholine-coated contact lens for extended wear use. Biomaterials. 2001;22(24):3261–72.View ArticleGoogle Scholar
- Yang W, et al. Pursuing “zero” protein adsorption of poly(carboxybetaine) from undiluted blood serum and plasma. Langmuir. 2009;25(19):11911–6.View ArticleGoogle Scholar
- Cheng G, et al. Zwitterionic carboxybetaine polymer surfaces and their resistance to long-term biofilm formation. Biomaterials. 2009;30(28):5234–40.View ArticleGoogle Scholar
- Cheng G, et al. Integrated antimicrobial and nonfouling hydrogels to inhibit the growth of planktonic bacterial cells and keep the surface clean. Langmuir. 2010;26(13):10425–8.View ArticleGoogle Scholar
- Cheng G, et al. A switchable biocompatible polymer surface with self-sterilizing and nonfouling capabilities. Angewandte Chemie. 2008;120(46):8963–6.View ArticleGoogle Scholar
- Chang Y, et al. Hemocompatible mixed-charge copolymer brushes of pseudozwitterionic surfaces resistant to nonspecific plasma protein fouling. Langmuir. 2010;26(5):3522–30.View ArticleGoogle Scholar
- Yang W, et al. Film thickness dependence of protein adsorption from blood serum and plasma onto poly(sulfobetaine)-grafted surfaces. Langmuir. 2008;24(17):9211–4.View ArticleGoogle Scholar
- Li G, et al. Ultra low fouling zwitterionic polymers with a biomimetic adhesive group. Biomaterials. 2008;29(35):4592–7.View ArticleGoogle Scholar
- Zhang Z, Chen S, Jiang S. Dual-functional biomimetic materials: nonfouling poly(carboxybetaine) with active functional groups for protein immobilization. Biomacromolecules. 2006;7(12):3311–5.View ArticleGoogle Scholar
- Xue C-H, et al. Fabrication of robust and antifouling superhydrophobic surfaces via surface-initiated atom transfer radical polymerization. ACS Appl Mater Interfaces. 2015;7(15):8251–9.View ArticleGoogle Scholar
- Privett BJ, et al. Antibacterial fluorinated silica colloid superhydrophobic surfaces. Langmuir. 2011;27(15):9597–601.View ArticleGoogle Scholar
- Li J, et al. Hydrophobic liquid-infused porous polymer surfaces for antibacterial applications. ACS Appl Mater Interfaces. 2013;5(14):6704–11.View ArticleGoogle Scholar
- Harrison RG. On the stereotropism of embryonic cells. Science. 1911;43(870):279–81.Google Scholar
- Recum AFV, et al. Surface roughness, porosity, and texture as modifiers of cellular adhesion. Tissue Eng. 1996;2(4):241–53.View ArticleGoogle Scholar
- Curtis A, Varde M. Control of cell behavior: topological factors. J Natl Cancer Inst. 1964;33(1):15–26.Google Scholar
- Korman N, Sudilovsky O, Gibbons D. The effect of humoral components on the cellular response to textured and nontextured PTFE. J Biomed Mater Res. 1984;18(2):225–41.View ArticleGoogle Scholar
- Curtis A, Wilkinson C. Topographical control of cells. Biomaterials. 1997;18(24):1573–83.View ArticleGoogle Scholar
- Chen CS, et al. Geometric control of cell life and death. Science. 1997;276(5317):1425–8.View ArticleGoogle Scholar
- Bettinger CJ, Langer R, Borenstein JT. Engineering substrate topography at the micro‐and nanoscale to control cell function. Angew Chem Int Ed. 2009;48(30):5406–15.View ArticleGoogle Scholar
- Xu L-C, Siedlecki CA. Submicron-textured biomaterial surface reduces staphylococcal bacterial adhesion and biofilm formation. Acta Biomater. 2012;8(1):72–81.View ArticleGoogle Scholar
- Kirschner CM, Brennan AB. Bio-inspired antifouling strategies. Annu Rev Mater Res. 2012;42(1):211–29.View ArticleGoogle Scholar
- Widawski G, Rawiso M, Francois B. Self-organized honeycomb morphology of star-polymer polystyrene films. Nature. 1994;369(6479):387–9.View ArticleGoogle Scholar
- Böltau M, et al. Surface-induced structure formation of polymer blends on patterned substrates. Nature. 1998;391(6670):877–9.View ArticleGoogle Scholar
- Lim JY, et al. Human foetal osteoblastic cell response to polymer-demixed nanotopographic interfaces. J R Soc Interface. 2005;2(2):97–108.View ArticleGoogle Scholar
- Karthaus O, et al. Formation of ordered mesoscopic patterns in polymer cast films by dewetting. Thin Solid Films. 1998;327:829–32.View ArticleGoogle Scholar
- Murthy N, et al. Self-assembled and etched cones on laser ablated polymer surfaces. J Appl Phys. 2006;100(2):023538.View ArticleGoogle Scholar
- Nishimoto S, Bhushan B. Bioinspired self-cleaning surfaces with superhydrophobicity, superoleophobicity, and superhydrophilicity. RSC Advances. 2013;3(3):671–90.View ArticleGoogle Scholar
- Chandra P, et al. UV laser-ablated surface textures as potential regulator of cellular response. Biointerphases. 2010;5(2):53–9.View ArticleGoogle Scholar
- Hoipkemeier-Wilson L, et al. Antifouling potential of lubricious, micro-engineered, PDMS elastomers against zoospores of the green fouling alga Ulva (Enteromorpha). Biofouling. 2004;20(1):53-63.Google Scholar
- Bixler GD, Bhushan B. Bioinspired rice leaf and butterfly wing surface structures combining shark skin and lotus effects. Soft Matter. 2012;8(44):11271–84.View ArticleGoogle Scholar
- Reddy ST, et al. Micropatterned surfaces for reducing the risk of catheter-associated urinary tract infection: an in vitro study on the effect of sharklet micropatterned surfaces to inhibit bacterial colonization and migration of uropathogenic Escherichia coli. J Endourol. 2011;25(9):1547–52.View ArticleGoogle Scholar
- Cheng YT, et al. Effects of micro- and nano-structures on the self-cleaning behaviour of lotus leaves. Nanotechnology. 2006;17(5):1359.View ArticleGoogle Scholar
- Koch K, Barthlott W. Superhydrophobic and superhydrophilic plant surfaces: an inspiration for biomimetic materials. Philos T Roy Soc A. 2009;367(1893):1487–509.View ArticleGoogle Scholar
- Ensikat HJ, et al. Superhydrophobicity in perfection: the outstanding properties of the lotus leaf. Beilstein J Nanotechnol. 2011;2(1):152–61.View ArticleGoogle Scholar
- Scardino A, et al. Biomimetic characterisation of key surface parameters for the development of fouling resistant materials. Biofouling. 2009;25(1):83–93.View ArticleGoogle Scholar
- Bers AV, Wahl M. The influence of natural surface microtopographies on fouling. Biofouling. 2004;20(1):43–51.View ArticleGoogle Scholar
- Carman ML, et al. Engineered antifouling microtopographies – correlating wettability with cell attachment. Biofouling. 2006;22(1):11–21.View ArticleGoogle Scholar
- Mann EE, et al. Surface micropattern limits bacterial contamination. Antimicrob Resist Infect Control. 2014;3(1):1.View ArticleGoogle Scholar
- Bers A, et al. Relevance of mytilid shell microtopographies for fouling defence–a global comparison. Biofouling. 2010;26(3):367–77.View ArticleGoogle Scholar
- Zhang L, Zhao N, Xu J. Fabrication and application of superhydrophilic surfaces: a review. J Adhes Sci Technol. 2014;28(8–9):769–90.View ArticleGoogle Scholar
- Zhang J, Severtson SJ. Fabrication and use of artificial superhydrophilic surfaces. J Adhes Sci Technol. 2014;28(8–9):751–68.View ArticleGoogle Scholar